See Section 2.2.1.

2.2.

See Section 2.1.

2.3.

See Section 2.1.1.

2.4.

See Section 2.1.1.

2.5.

See Section 2.1.2.

2.6.

See Section 2.2.1.

2.7.

See Section 2.1.2.

2.8.

See Section 2.2.1.

2.9.

See Section 2.2.1.

2.10. If the atomic masses and radii are the same, then the material that crystalizes into a lattice with a higher APF will have a larger density. The FCC structure has a higher APF than the BCC structure.

2.11. For the face-center cubic crystal structure, number of equivalent whole atoms in each unit cell = 4 By inspection the diagonal of the face of a FCC unit cell = 4r

Using Pythagorean theory: (4r)2 = a2 + a2 16r2 = 2 a2 8r2 = a2 a 2 2r

2.12. a. Number of equivalent whole atoms in each unit cell in the BCC lattice structure = 2 b. Volume of the sphere = (4/3) r3

Volume of atoms in the unit cell = 2 x (4/3) r3 = (8/3) r3 By inspection, the diagonal of the cube of a BCC unit cell = 4r = a 2 a 2 a 2 =a 3 a = Length of each side of the unit cell =

4r 3

4r 

3

c. Volume of the unit cell = APF

volume of total

3 atoms in the unit

unit

volume of

cell

=

(8 / 3) .r

3

= 0.68

(4r / 3) 3

the cell

4r 3

2.13. For the BCC lattice structure: a

3

r Volume of the unit cell of iron =

4

3

4x0.124x109

= 2.348 x 10-29 m3

=  3

3

2.14. For the FCC lattice structure: a 2 2r Vol. of unit cell of aluminum = (2 2r) 3 = (2 2x0.143) 3 =0.06616725 nm3 = 6.6167x10 -29 m3

2.15. From Table 2.3, copper has an FCC lattice structure and r of 0.1278 nm 3 3 Volume of the unit cell of copper = (2 2r) = (2 2x0.1278) = 0.04723 nm3 = 4.723 x10 -29 m3 2.16. For the BCC lattice structure: a

4r 3 3

r Volume of the unit cell of iron =

4

4x0.124x109

= 2.348 x 10-29 m3

=  3

3 Density =

3

nA VC NA

n = Number of equivalent atoms in the unit cell = 2 A = Atomic mass of the element = 55.9 g/mole NA= Avogadro’s number = 6.023 x 1023 2 x55.9 = 7.904 x 106 g/m3 = 7.904 Mg/m3 29 23 2.348x10 x6.023x10

2.17. For the BCC lattice structure: a

4r 3 3

Vol. of the unit cell of molybdenum =

4r 

=

4 x0.1363x10 9 

3

= 3.119 x 10-29 m3

3 nA

=

2 x95.94 29

3.119x10 x6.023x10 VC NA

3

ï&#x20AC;

10.215 x 106 g/m3= 10.215 Mg/ m3

23

2.18.

4r 3

For the BCC lattice structure: a

3

4r 

Volume of the unit cell of the metal =

=

3 nA

=

2 x63.5

4 x0.128x10 9  3

3

= 2.583 x 10-29 m3

8.163 x 106 g/m3= 8.163 Mg/ m3

29

2.583x10 x6.023x10

23

VC NA 2.19. For the FCC lattice structure: a 2 2r Volume of unit cell of the metal = (2 2r) 3 = (2 2 x0.132) 3 =0.05204 nm3 = 5.204x10-29 m3 nA

=

4 x42.9 29

5.204x10 x6.023x10

5.475 x 106 g/m3= 5.475 Mg/ m3

23

VC NA 2.20. For the FCC lattice structure: a 2 2r Volume of unit cell of aluminum = (2 2r) 3 = (2 2x0.143) 3 =0.06616725 nm3 = 6.6167x10-29 m3 nA Density = 

VC N A For FCC lattice structure, n = 4 A = Atomic mass of the element = 26.98 g/mole NA= Avogadro’s number = 6.023 x 1023 4x26.98 = 2.708 x 106 g/m3 = 2.708 Mg/m3 6.6167 x10 29 x6.023x10 23 2.21.

nA VC NA For FCC lattice structure, n = 4 4x63.55 = 4.747 x 10-29 m3 8.89x10 6 x6.023x10 23 4x(4 / 3) .r 3 APF = 0.74 = 4.747 x10 29 r3 = 0.2097 x 10-29 m3 r =0.128 x 10-9 m = 0.128 nm

Vc =

2.22. a.

nA VC NA For FCC lattice structure, n = 4 4x40.08 Vc = = 1.717 x 10-28 m3 1.55x10 6 x6.023x10 23

4x(4 / 3) .r 3 b. APF = 0.74 = 1.717 x10 28

r3 = 0.7587 x 10-29 m3 r =0.196 x 10-9 m = 0.196 nm 2.23.

2.24. See Section 2.2.2. 2.25. See Section 2.2.2. 2.26. See Section 2.2.2. 2.27. See Figure 2.14. 2.28. See Section 2.2.5. 2.29. mt = 100 g PB = 65 % PlB = 30 % PsB = 80 % From Equations 2.4 and 2.5, ml + ms = 100 30 ml+ 80 ms = 65 x 100 Solving the two equations simultaneously, we get: ml = mass of the alloy which is in the liquid phase = 30 g ms = mass of the alloy which is in the solid phase = 70 g 2.30. mt = 100 g PB = 45 % PlB = 17 % PsB = 65 % From Equations 2.4 and 2.5, ml + ms = 100 17 ml+ 65 ms = 45 x 100 Solving the two equations simultaneously, we get: ml = mass of the alloy which is in the liquid phase = 41.67 g ms = mass of the alloy which is in the solid phase = 58.39 g

2.31. mt = 100 g PB = 60 % PlB = 25 % PsB = 70 % From Equations 2.4 and 2.5, ml + ms = 100 25 ml+ 70 ms = 60 x 100 Solving the two equations simultaneously, we get: ml = mass of the alloy which is in the liquid phase = 22.22 g ms = mass of the alloy which is in the solid phase = 77.78 g 2.32. mt = 100 g PB = 40 % PlB = 20 % PsB = 50 % From Equations 2.4 and 2.5, ml + ms = 100 40 ml+ 50 ms = 40 x 100 Solving the two equations simultaneously, we get: ml = mass of the alloy which is in the liquid phase = 33.33 g ms = mass of the alloy which is in the solid phase = 66.67 g 2.33. a. Spreading salt reduces the melting temperature of ice. For example, at a salt composition of 5%, ice starts to melt at -21oC. When temperature increases more ice will melt. At a temperature of -5oC, all ice will melt. b. -21oC c. -21oC 2.34.

See Section 2.3.

2.35.

See Section 2.3.

2.36.

See Section 2.4.